Microstructure and mechanical properties of disperse Ni£¢ ... surface roughness and...
Embed Size (px)
Transcript of Microstructure and mechanical properties of disperse Ni£¢ ... surface roughness and...
A R R 1 A
K A N X M
a a w [ f T t [ c e t
Materials Chemistry and Physics 120 (2010) 409–416
Contents lists available at ScienceDirect
Materials Chemistry and Physics
journa l homepage: www.e lsev ier .com/ locate /matchemphys
icrostructure and mechanical properties of disperse Ni–Co alloys lectrodeposited on Cu substrates
.D. Rafailović a, H.P. Karnthalera, T. Trišović b, D.M. Minić c,∗
University of Vienna, Physics of Nanostructured Materials, Faculty of Physics, Boltzmanngasse 5, 1090 Vienna, Austria Institute of Technical Sciences of Serbian Academy of Science and Arts, Knez Mihailova 35, Belgrade, Serbia University of Belgrade, Faculty of Physical Chemistry, Studentski trg 12, 11000, Belgrade, Serbia
r t i c l e i n f o
rticle history: eceived 12 April 2009 eceived in revised form 0 November 2009 ccepted 19 November 2009
eywords: lloys anostructured materials -ray scattering icrostructure
a b s t r a c t
The nickel and cobalt disperse alloy deposits of five different compositions were obtained by electrode- position on Cu substrates in the galvanostatic regime from an ammonium sulfate-chloride solution. The effect of cathodic current density and Ni2+/Co2+ ions concentration ratio in the electrolyte on the composition, microstructure, morphology and mechanical properties of Ni–Co alloys were investigated. Conditions for formation of nanostrustured disperse deposits and surface roughness was determined by 3D SEM reconstruction of the specimen surface. It was established that formation of the disperse deposits with highly developed structures is favored from bath with equal Ni2+/Co2+ ions concentration ratio in the electrolyte. Cathodic polarization diagrams determined for all investigated alloys have shown shift of the cathodic potential for alloy deposition to the more negative values with increasing Ni2+/Co2+ ions concentration ratio in the electrolyte. An increase of in the cobalt content in the alloy was observed with decreasing the current density and increasing of the Co2+ ions concentration ratio in the bath. X-ray analyses of nanocrystalline Ni–Co deposits show formation of a single phase face-centered cubic (FCC), a
single phase hexagonal-close packed (HCP) and mixture of FCC solid solutions and HCP phase depending on the current density applied and electrolyte composition. The increase of HCP phase content in the nanocrystalline deposits appears as a result of both, the increase in Co2+ ions concentration in the bath and decrease of deposition current density. The mechanical properties of nanocrystalline deposits have shown increase of the hardness with increasing Ni content in the alloy. The cross-section of the samples
bstra he be
electrodeposited on Cu su density values revealed t
The recent interest in the electrodeposition of iron-group met- ls (Ni, Co and Fe) and their alloys is due to their unique magnetic nd thermophysical properties [1,2]. Electrodeposition is a process hich is capable for depositing nanocrystalline metals and alloys
3] onto recessed and non-uniform surfaces, and therefore has ound a role in microelectromechanical systems (MEMS) [2,4–7]. he hardness and strength of the electrolytic deposits are bet- er than alloys prepared by conventional metallurgical processes 2]. One of the most important aspects of electrodeposition pro- ess is possibility for production of nanocrystalline materials which
xhibit unique properties compared to the microcrystalline coun- erparts .
A metal powder represents a loose deposit which can sponta- eously fall off from the electrode or can be removed by tapping or
∗ Corresponding author. E-mail addresses: firstname.lastname@example.org, email@example.com (D.M. Minić).
254-0584/$ – see front matter © 2009 Elsevier B.V. All rights reserved. oi:10.1016/j.matchemphys.2009.11.029
tes from electrolytes with equal ion metal concentration at lower current ginning of a dendrite structure formation.
© 2009 Elsevier B.V. All rights reserved.
by other similar way [8–10]. The electrodeposition of the powders from the solutions, established by the work of Calusaru  pos- sesses significant advantages over other methods for synthesis of nanocrystalline materials . This method usually yields products of requested chemical composition and high purity, which can be well pressed and sintered [12–14]. The effect of operating condi- tions, electrolyte composition, temperature and pH on the Ni–Co composition and properties of obtained deposits are widely inves- tigated [15–18]. On the other hand, electrodeposition at very high current density and high overpotential is only investigated for the case of the obtaining of powders [19–21].
However, electrochemical synthesis of disperse deposits on the substrate is insufficiently investigated . Investigations of such Cu deposits formed at high current densities characterized by open and very porous structures with extremely high surface
areas were initiated recently . It has been stated that the open and porous structures of copper deposits obtained at high current densities were ideally suited for use as electrodes in electrochem- ical devices such as fuel cells, batteries and chemical sensors , while the extremely high surface area is relevant for evaluating
http://www.sciencedirect.com/science/journal/02540584 http://www.elsevier.com/locate/matchemphys mailto:firstname.lastname@example.org mailto:email@example.com dx.doi.org/10.1016/j.matchemphys.2009.11.029
4 mistry and Physics 120 (2010) 409–416
s a d l d ( T o d m s
u c C g m t 0 a w t
e a p d c f a
c 2 I b
s r w i a u r ( 0
n o q c O
t o p t t t
s t c t
Fig. 1. Polarization curves for the cathodic process of Ni–Co deposition on cop-
where the disperse deposits were obtained, the current efficiency decreases with the increase of the current density and with the decrease of the Ni2+ concentration in the electrolyte.
10 L.D. Rafailović et al. / Materials Che
ome electrochemical reactions . Surface microstructure plays crucial role in application such as a magnetic storage, printing
evices and all other similar technological procedures, but corre- ation between surface morphology and roughness structure with eposition parameters is still open topic . Three-dimensional 3D) characterization seems more adapted for applied research. herefore, the aim of this study is investigation of the influence f deposition current density on microstructure of disperse Ni–Co eposits and correlation between electrolysis conditions for for- ation of such rough deposits on the substrates with morphology,
urface roughness and mechanical properties.
The deposits were obtained in an open glass electrochemical cell with a vol- me of 1 dm3, thermostatically controlled at a temperature of 298 K. A Ti-plate overed with RuO2/TiO2 (10 cm2 geometric area), placed close and parallel to the u plate, was used as an anode (DSA). The solutions were made from analytical rade chemicals and triple distilled water. The alloys were electrodeposited from ixed ammonium sulfate-chloride solutions of different Ni2+/Co2+ ions concen-
ration ratios of 0.25, 0.5, 1, 2 and 4 (total concentration of NiSO4 + CoSO4 was .12 mol dm−3) using 0.5 mol dm−3 NH4Cl and 3.5 mol dm−3 NH4OH as a buffering gent and a supporting electrolyte at pH 10. The electrodeposition was performed ith a constant current regime ranging from 65 to 400 mA cm−2. The deposition
ime was adjusted to the same quantity of electricity (43 mA cm−2). Polarization diagrams were recorded with the three-compartment standard
lectrochemical cell at a temperature of 298 K. The platinum foil counter electrode nd the reference–saturated calomel electrode (SCE) were placed at separate com- artments, connected to the working electrode by a Luggin capillary positioned at a istance of 0.2 cm from the working electrode surface. The working electrode was a opper electrode rod (d = 0.4 cm). Before each experiment the working electrode sur- ace was polished using 0.05 �m alumina impregnated polishing cloths. The Ni–Co lloys were electrodeposited with same quantity of electricity (43 mAh cm−2).
Polarization measurements were performed by a computer controlled electro- hemical system (PAR M 273A) using the corrosion software (PAR M352/252, version .01) with a sweep rate of 1 mV s−1. To obtain polarization curves corrected for the R drop, current interrupt technique was used with the time of current interruption eing 0.5 s.
The current efficiency of alloy deposits was determined at different current den- ities by measuring the mass of the deposit on the copper cathode which was used s a working electrode.
Surface morphology was examined using an XL 30 ESEM-FEG (environmental canning electron microscope with field emission gun, FEI Company, NL). The 3D econstruction of the specimen surface was characterized by SEM using MeX soft- are from Alicona (A). It enables to carry out a 3D analysis directly from the digital
mages yielding profile and roughness measurements and also area analysis as well s volumetric measurements. An alloy composition analysis was performed by ESEM sing the energy dispersive X-ray spectrometry (EDX) software Genesis (USA). X- ay powder diffraction (XRD) analysis was carried out using a MPD diffractometer Philips, NL) with CuK� radiation (40 kV/30 mA). Step scan mode was u